Microstructural Evolution of Calcium Sulfoaluminate Cement during the Wet-Carbonation Process

: Calcium sulfoaluminate (CSA) cement, as a type of low-carbon cement, can contribute to further reduction in carbon emissions with carbonation technologies. However, the detailed microstructure development of CSA cement during the carbonation process has been rarely analyzed. In this paper, wet carbonation was applied to CSA cement to investigate the microstructure evolution of carbonation products and carbon absorption capacity of CSA cement by means of pH measurement, X-ray diffraction (XRD) measurement


Introduction
Nowadays, the annual production of Portland cement in China is approximately 2.4 billion tons, ranking first in the world.However, approximately 0.9 t CO 2 is released during the production of 1t Portland cement, making the cement industry an important source of carbon emissions [1][2][3].It is reported that the carbon emissions of the Portland cement industry around the world have accounted for approximately 26% of the total industrial carbon emissions and approximately 7% of the total human carbon emissions.Therefore, in order to achieve China's strategic goals of "carbon neutrality and peak carbon emissions", it is urgent to reduce carbon emissions from the cement industry [4].Carbon capture, utilization and storage (CCUS) technology has been proposed recently to prevent excessive carbon emissions, which includes three main processes: CO 2 capture, utilization and storage.CO 2 capture is the separation and collection of CO 2 from factory emission sources; CO 2 utilization refers to the use of captured CO 2 for the manufacture of new products; CO 2 storage is the storage of captured CO 2 underground [5,6].Researchers are constantly exploring better applications of CCUS technology in the cement and concrete industry [7,8].
Calcium sulfoaluminate cement (CSA cement), as the third series of cement independently developed in China, has become a highly promising low-carbon cement due to its advantages of low calcination temperature, low consumption of limestone as raw materials and easy wear resistance [9][10][11][12].In addition, CSA cement has high early strength, good impermeability and frost resistance and micro-expansion characteristics.It has also been successfully applied in emergency repair and construction, marine construction and other projects [4,13,14].Ye'elimite (C 4 A 3 Š) and belite (C 2 S) are the main minerals in CSA cement: The former enables this type of cement to have quick hardening speed and early strength on account of its rapid hydration, and the latter provides later strength owing to the C-S-H gel generated at the later age.Generally, the hydration of C 4 A 3 Š occurs according to Equation (1) to generate monosulfate (C 4 AŠH 12 ) and aluminum hydroxide (AH 3 ) gel.Under the circumstances of excessive water, C 3 AH 6 may form according to Equation (2).Actually, during the manufacture of CSA cement, gypsum (CŠH 2 ) or anhydrite is used, and C 4 A 3 Š will react with calcium sulfate to generate ettringite (C 6 AŠH 32 ) and AH 3 (Equation ( 3)).Moreover, the hydration of C 2 S tends to generate C-S-H and portlandite (CH) according to Equation (4).With the hydration of C 4 A 3 Š and C 2 S at the same time, C 2 S will react with AH 3 to generate str 2 of 15 ture, utilization and storage (CCUS) technology has been proposed recently xcessive carbon emissions, which includes three main processes: CO2 capture, and storage.CO2 capture is the separation and collection of CO2 from factory urces; CO2 utilization refers to the use of captured CO2 for the manufacture of cts; CO2 storage is the storage of captured CO2 underground [5,6].Researchers tly exploring better applications of CCUS technology in the cement and contry [7,7,8].m sulfoaluminate cement (CSA cement), as the third series of cement indeeveloped in China, has become a highly promising low-carbon cement due to ges of low calcination temperature, low consumption of limestone as raw nd easy wear resistance [9][10][11][12].In addition, CSA cement has high early od impermeability and frost resistance and micro-expansion characteristics.been successfully applied in emergency repair and construction, marine connd other projects [4,13,14].Ye'elimite (C4A3Š) and belite (C2S) are the main CSA cement: The former enables this type of cement to have quick hardening early strength on account of its rapid hydration, and the latter provides later ing to the C-S-H gel generated at the later age.Generally, the hydration of rs according to Equation (1) to generate monosulfate (C4AŠH12) and aluminum (AH3) gel.Under the circumstances of excessive water, C3AH6 may form ac-Equation (2).Actually, during the manufacture of CSA cement, gypsum anhydrite is used, and C4A3Š will react with calcium sulfate to generate 6AŠH32) and AH3 (Equation ( 3)).Moreover, the hydration of C2S tends to -S-H and portlandite (CH) according to Equation (4).With the hydration of 2S at the same time, C2S will react with AH3 to generate strȁtlingite (C2ASH8) 5)).(2) the carbonation of CSA cement, most of the studies have focused on its meoperty, such as compressive strength, expansion, etc. [15][16][17][18][19][20][21].For instance, ation, the mechanical property of CSA cement was improved as reported by 2], but it was also influenced by the water-to-cement ratio.Moreover, differtion methods usually present various results, e.g., a carbonation chamber is d for carbonation, and thus, the difference between the accelerated carbonaenvironmental carbonation can be investigated.Seo [20] studied CSA cement pplemented with different amounts of MgO, and after hydration for 56 d, the re carbonated for studying compressive strength; the result showed that the sage of MgO was 10 wt.% for improvement of strength.By mixing with slag, ical property of CSA cement can be promoted after being exposed to CO2 for bonation [23].Regarding the microstructure during the carbonation of CSA was found that, after ettringite was entirely carbonated, the carbonation ainly consisted of gypsum and calcium carbonate (in three polymorphs, i.e., onite and vaterite), which has been found with the XRD results reported by staldia [19].Also, the carbonation of CSA cement supplemented with PC was tlingite (C 2 ASH 8 ) (Equation ( 5)).
As for the carbonation of CSA cement, most of the studies have focused on its mechanical property, such as compressive strength, expansion, etc. [15][16][17][18][19][20][21].For instance, after carbonation, the mechanical property of CSA cement was improved as reported by Mechling [22], but it was also influenced by the water-to-cement ratio.Moreover, different carbonation methods usually present various results, e.g., a carbonation chamber is usually used for carbonation, and thus, the difference between the accelerated carbonation and the environmental carbonation can be investigated.Seo [20] studied CSA cement that was supplemented with different amounts of MgO, and after hydration for 56 d, the samples were carbonated for studying compressive strength; the result showed that the optimal dosage of MgO was 10 wt.% for improvement of strength.By mixing with slag, the mechanical property of CSA cement can be promoted after being exposed to CO 2 for further carbonation [23].Regarding the microstructure during the carbonation of CSA cement, it was found that, after ettringite was entirely carbonated, the carbonation products mainly consisted of gypsum and calcium carbonate (in three polymorphs, i.e., calcite, aragonite and vaterite), which has been found with the XRD results reported by Daniela Gastaldia [19].Also, the carbonation of CSA cement supplemented with PC was reported, and the carbonation of monosulfate was revealed rather than ettringite, as the ettringite content was not substantially decreased, and the generation of gypsum was attributed to the carbonation of monosulfate [19].For the carbonation of CSA cement, the sample was normally hydrated for a certain number of days (28 d or 56 d) and then put into a carbonation chamber for research.This means that the traditional carbonation method applied for CSA cement was a method of hydration followed by carbonation.
As an important carbonation method, wet carbonation has always been in the stage of continuous development and deep exploration.The contact area and dissolution rate of CO 2 can be increased with wet carbonation, which is helpful to simulate and observe the carbonation process in a short time [24].Researchers are dedicated to studying the kinetics and thermodynamics of the interaction between cement components and CO 2 as well as the impact of different environmental conditions (temperature, humidity, pressure, etc.) on carbonation.Additionally, the mechanical properties and microstructure of cement or concrete after carbonation are evaluated.For instance, the impacts of gas pressure, water-to-solid ratio, gas-to-liquid ratio and reaction time on CO 2 absorption were assessed by introducing cement plant flue gas into discarded concrete [25].The results indicate that increasing the total gas pressure, gas-liquid ratio and liquid-solid ratio is an effective method to enhance the efficiency of mineral carbonation.By using waste CO 2 to wet carbonated recycled concrete aggregate (RAC) and recycled concrete fine particles (RCF), the purposes of absorbing more carbon dioxide and improving the material properties would be achieved [26,27].The wet-carbonation process was characterized in detail, revealing changes in the microstructures (such as pores and carbonation products), compressive strength and other mechanical properties.This approach demonstrates the advantages of efficient and low-energy wet carbonation.Direct carbonation of synthetic concrete powder was achieved by controlling various solid-to-liquid ratios (10, 25 and 50 g/L) and different concentrations of CO 2 (5%, 14% and 30%).Characterization involves assessing the carbonation products, CO 2 absorption capacity and crystalline structure of the resulting calcium carbonate [24].
In general, the carbonation of CSA cement was previously studied with dry carbonation or environmental carbonation, where CSA cement was hydrated first and then exposed to CO 2 .Therefore, in this work, wet carbonation was applied in the carbonation of CSA cement to study the coupling mechanism of hydration and carbonation reactions, and the corresponding microstructure evolution was investigated.The wet carbonation applied in CSA cement can be revealed for guidelines of the carbonation mechanism of CSA cement.By means of XRD, TG and FT-IR, the evolution of the microscopic phases was studied, and the microstructure was displayed from SEM images.Also, thermodynamic modeling was conducted for further explanation.

Raw Materials and Characterization
In this work, a fast-hardening calcium sulfoaluminate cement was used.The chemical compositions of the CSA cement used in this study are as follows: 13.86

Wet-Carbonation Process
The same batch of cement with the same particle size was used in this work.T experiment was carried out in a special reaction device, as shown in Figure 2. CSA ment and deionized water were added to the beaker with a mass ratio of 1/20 at ro temperature, and the mixed paste was stirred in the beaker for 10 min for a stable value.The speed of stirring was constantly kept at 200 rpm.CO2 with a 99.9% concen tion was injected into the solution through a sparkling stone at a flow rate of 150 mL/m and the pressure of CO2 was maintained at 0.2 MPa throughout the entire process.Sa ples with different carbonation times of 10 s, 30 s, 1 min, 2 min, 5 min, 10 min, 15 min min, 30 min, 1 h, 2 h, 12 h and 24 h were prepared as separate batches.After a cert period of carbonation, the carbonated samples were filtered first, and isopropanol w used for the termination of both carbonation and hydration.After filtering, these samp were dried in a vacuum drier for 8 min at 40 °C [28].

Wet-Carbonation Process
The same batch of cement with the same particle size was used in this work.The experiment was carried out in a special reaction device, as shown in Figure 2. CSA cement and deionized water were added to the beaker with a mass ratio of 1/20 at room temperature, and the mixed paste was stirred in the beaker for 10 min for a stable pH value.The speed of stirring was constantly kept at 200 rpm.CO 2 with a 99.9% concentration was injected into the solution through a sparkling stone at a flow rate of 150 mL/min, and the pressure of CO 2 was maintained at 0.2 MPa throughout the entire process.Samples with different carbonation times of 10 s, 30 s, 1 min, 2 min, 5 min, 10 min, 15 min, 20 min, 30 min, 1 h, 2 h, 12 h and 24 h were prepared as separate batches.After a certain period of carbonation, the carbonated samples were filtered first, and isopropanol was used for the termination of both carbonation and hydration.After filtering, these samples were dried in a vacuum drier for 8 min at 40

Wet-Carbonation Process
The same batch of cement with the same particle size was used in this wor experiment was carried out in a special reaction device, as shown in Figure 2. C ment and deionized water were added to the beaker with a mass ratio of 1/20 at temperature, and the mixed paste was stirred in the beaker for 10 min for a sta value.The speed of stirring was constantly kept at 200 rpm.CO2 with a 99.9% conc tion was injected into the solution through a sparkling stone at a flow rate of 150 m and the pressure of CO2 was maintained at 0.2 MPa throughout the entire process ples with different carbonation times of 10 s, 30 s, 1 min, 2 min, 5 min, 10 min, 15 m min, 30 min, 1 h, 2 h, 12 h and 24 h were prepared as separate batches.After a c period of carbonation, the carbonated samples were filtered first, and isopropan used for the termination of both carbonation and hydration.After filtering, these sa were dried in a vacuum drier for 8 min at 40 °C [28].

pH Measurement
All carbonated samples were filtered to obtain filter residue and solution.The pH of each filtrate was measured with a pH meter (model REX PHS-3C).

X-ray Diffraction (XRD) Measurement
The crystalline phase was analyzed with Rigaku SmartLab, an intelligent X-ray polycrystalline diffractometer.During the test, the working voltage was 45 kV, the working current was 200 mA, and the scanning speed was set at 2 • /min with a range of 5-80 • 2θ.ZnO as the internal standard was added to the sample for the quantitative analysis [29][30][31][32].EVA V3.1 software was used to qualitatively analyze the XRD pattern and determine the product types.TOPAS 4.2 software was used to quantitatively analyze the XRD pattern and determine the content of each phase.

Thermogravimetric (TG) Measurement
The TG-DTG of the samples with different carbonation times was measured with a Hitachi Limited thermogravimetric analyzer.The test temperature ranged from 30 • C to 1000 • C. The heating rate was 10 • C/min, and the N 2 atmosphere was kept at the speed of 40 mL/min.

Fourier-Transformed Infrared Spectroscopy (FT-IR) Measurement
The FT-IR spectroscopy was conducted with a Bruker INVENIO spectrometer.The resolution of the test was 4 cm −1 , and the scope of the data scan was from 4000 cm −1 to 400 cm −1 .In addition, each sample went through 32 scanning times.

Scanning Electron Microscope (SEM) Measurement
A TESCAN Vega3 was used to observe and analyze the morphology and particle size of each sample after carbonation.The carbonated powder was applied to the carbon glue, and gold was sprayed once through the SBC-12 ion sputtering meter, keeping the current at 10 mA.The operating software Vega TC was employed for scanning and analyzing.

GEMS Modeling
Gibbs free-energy minimization software (GEMS V3.7) was employed to predict the formation and transformation of the different phases involved in the cement carbonation reaction.The CEMDATA18 database dedicated to cement was used in the simulation process.The final stable products of CSA cement after hydration and carbonation were simulated as a reference for the experiment.

pH Analysis
Figure 3 shows the pH value at the different carbonation times of 10 s, 30 s, 1 min, 2 min, 5 min, 10 min, 15 min, 20 min, 30 min, 1 h, 2 h, 12 h and 24 h, respectively.After carbonation for 30 s, the pH reached the maximum value of 10.5, which was probably linked to the hydration of CSA cement despite the addition of CO 2 .As reported before, the pH value of hydrated cement paste always ranges from 12 to 13 [33].Although the pH value had not reached 12 at 30 s, it could be considered that the carbonic acid in the solution reduced the pH value.After carbonation for 1 min, the pH of the solution decreased rapidly, which can be attributed to the occurrence of the carbonation reaction along with the formation of carbonic acid.It is worth noting that, before 10 min, the pH of the solution was alkaline, which can be associated with the hydration of C 4 A 3 Š and C 2 S, but the pH of the solution was acidic after 10 min, owing to the excessive addition of CO 2 to form carbonic acid in the solution.Ultimately, the pH value of the solution tended to be stable beginning from 10 min.Generally, after exposure to a large amount of CO 2 , the pH showed an increased trend, followed by a decreased trend, which revealed the coupling interaction between the hydration and carbonation reactions [21,[34][35][36][37].
to form carbonic acid in the solution.Ultimately, the pH value of the solution tended to be stable beginning from 10 min.Generally, after exposure to a large amount of CO2, the pH showed an increased trend, followed by a decreased trend, which revealed the coupling interaction between the hydration and carbonation reactions [21,[34][35][36][37].

XRD Analysis
The XRD patterns of the carbonated samples are shown in Figure 4.The main components of CSA cement, i.e., C4A3Š, C2S and anhydrite, can be observed with the XRD diffraction peaks throughout the entire process.With the increasing carbonation time, the diffraction peaks of C4A3Š and C2S gradually weakened.The diffraction peaks of gibbsite, one of the hydration products of C4A3Š [37], can be detected throughout the carbonation process.The diffraction peaks of ettringite were not visible, owing to its carbonation reaction.On the other hand, as the pH rapidly diminished, it was difficult for the ettringite to exist stably in this pH environment [38].

XRD Analysis
The XRD patterns of the carbonated samples are shown in Figure 4.The main components of CSA cement, i.e., C 4 A 3 Š, C 2 S and anhydrite, can be observed with the XRD diffraction peaks throughout the entire process.With the increasing carbonation time, the diffraction peaks of C 4 A 3 Š and C 2 S gradually weakened.The diffraction peaks of gibbsite, one of the hydration products of C 4 A 3 Š [37], can be detected throughout the carbonation process.The diffraction peaks of ettringite were not visible, owing to its carbonation reaction.On the other hand, as the pH rapidly diminished, it was difficult for the ettringite to exist stably in this pH environment [38].
stable beginning from 10 min.Generally, after exposure to a large amount of CO2, the pH showed an increased trend, followed by a decreased trend, which revealed the coupling interaction between the hydration and carbonation reactions [21,[34][35][36][37].

XRD Analysis
The XRD patterns of the carbonated samples are shown in Figure 4.The main components of CSA cement, i.e., C4A3Š, C2S and anhydrite, can be observed with the XRD diffraction peaks throughout the entire process.With the increasing carbonation time, the diffraction peaks of C4A3Š and C2S gradually weakened.The diffraction peaks of gibbsite, one of the hydration products of C4A3Š [37], can be detected throughout the carbonation process.The diffraction peaks of ettringite were not visible, owing to its carbonation reaction.On the other hand, as the pH rapidly diminished, it was difficult for the ettringite to exist stably in this pH environment [38].Generally, the primary distinction of the XRD diffraction peaks was calcium carbonate.After carbonation for 10 min, calcite, aragonite and vaterite began to generate, which can be associated with the carbonation of ettringite and the hydration products of belite [39].Regarding the samples carbonated for 10 s, there was no calcium carbonate generated, and it can be attributed to the formation of carbonic acid in the solution rather than the carbonation of ettringite or the hydration products of belite.Furthermore, after carbonation for 15 min, aragonite was no longer visible until carbonation for 24 h.It can be observed from the XRD pattern that calcite showed sharp characteristic diffraction peaks at 2θ degree of 29.2 • along with diffraction peaks at 2θ degree of 39.4 • , 43.2 • , 48.3 • and 57.5 • ; vaterite showed a diffraction peak at 2θ degree of 32.5 • , and aragonite showed a diffraction peak at a degree of 26.3 • .In addition, the peaks of C 4 A 3 Š and anhydrite varied with the of CO 2 , which possibly suggested the different hydration degree of C 4 A 3 Š and anhydrite.In Table 2, the QXRD analysis of each carbonated sample acquired with Rietveld quantification is given for further explanation.Figure 5 shows an example of the Rietveld plot.Generally, the primary distinction of the XRD diffraction peaks was calcium carbonate.After carbonation for 10 min, calcite, aragonite and vaterite began to generate, which can be associated with the carbonation of ettringite and the hydration products of belite [39].Regarding the samples carbonated for 10 s, there was no calcium carbonate generated, and it can be attributed to the formation of carbonic acid in the solution rather than the carbonation of ettringite or the hydration products of belite.Furthermore, after carbonation for 15 min, aragonite was no longer visible until carbonation for 24 h.It can be observed from the XRD pattern that calcite showed sharp characteristic diffraction peaks at 2θ degree of 29.2° along with diffraction peaks at 2θ degree of 39.4°, 43.2°, 48.3° and 57.5°; vaterite showed a diffraction peak at 2θ degree of 32.5°, and aragonite showed a diffraction peak at a degree of 26.3°.In addition, the peaks of C4A3Š and anhydrite varied with the amount of CO2, which possibly suggested the different hydration degree of C4A3Š and anhydrite.In Table 2, the QXRD analysis of each carbonated sample acquired with Rietveld quantification is given for further explanation.Figure 5 shows an example of the Rietveld plot.As observed in Table 2, the content of the two main components (C 4 A 3 Š and C 2 S) decreased significantly as the carbonation time increased, and the decrease of C 2 S was faster than that of C 4 A 3 Š since C 2 S is more prone to carbonation as reported before [30].The result that C 4 A 3 Š decreased before 15 min with no variation later suggested that both its hydration and carbonation occurred before 15 min, and later, the hydration of C 4 A 3 Š no longer proceeded, let alone the carbonation reaction; this result can be proved by the change in C 2 S, which showed a slight decrease before 15 min and a rapid reduction later.
After 24 h of carbonation, C 2 S was almost completely carbonated to generate different types of calcium carbonate.However, the decrease in C 4 A 3 Š exhibited a relatively low trend compared to C 2 S, as the formation of ettringite was inhibited in the acidic environment, and thus, the hydration of C 4 A 3 Š was indirectly inhibited as well.Meanwhile, the amount of anhydrite diminished as well, which can be attributed to its hydration with C 4 A 3 Š.Specifically, no ettringite was generated on account of its carbonation, and gypsum and calcium carbonate were generated as a result.Regarding the amount of gypsum, it can be concluded from Table 2 that its content reached a maximum value at 15 min and then diminished partly to the end.It can be ascribed to the presence of C 4 A 3 Š in the solution and the further reaction between C 4 A 3 Š and gypsum.In other words, the hydration of C 4 A 3 Š in the solution involved mainly two parts: One is the reaction with anhydrite, and the other is the reaction with the generated gypsum.These small amounts of gypsum reacted with C 4 A 3 Š to generate ettringite, which was immediately carbonated, and it further confirmed the carbonation of ettringite despite no obvious characteristics of ettringite in the XRD pattern.
The content of C 2 S decreased with increasing carbonation time, especially for carbonation for more than 15 min, indicating the occurrence of the carbonation reaction, whose carbonation mainly leads to the generation of calcium carbonate, as is observed from the XRD results and QXRD results.Among the three types of calcium carbonate, calcite increased rapidly at the early stage of carbonation (from 10 s) and gradually stabilized in the later stage.The content of calcite reached the maximum value at 10 min.Before 15 min, vaterite existed in a large amount, but its content gradually decreased after 15 min.In addition, aragonite was not detected until 24 h, which can be observed from the XRD result at 24 h.Although each content was relatively low, vaterite and aragonite still existed until C 2 S was entirely carbonated (the sample at 24 h).It is worth noting that the content of calcium carbonate also decreased slightly.In addition to calcite with good crystal form, poorly crystallized or amorphous calcium carbonate was also observed.As shown in Table 2, the amorphous content was increasing.As for gibbsite, its quantity reached the maximum value after being exposed to CO 2 for 1 h, which proved the coupling interaction between the hydration and carbonation reactions as well; and the amount of gibbsite decreased after 12 h, which was probably associated with its reaction with C 2 S and the further carbonation of the formed str 2 of 15 re, utilization and storage (CCUS) technology has been proposed recently essive carbon emissions, which includes three main processes: CO2 capture, storage.CO2 capture is the separation and collection of CO2 from factory ces; CO2 utilization refers to the use of captured CO2 for the manufacture of ; CO2 storage is the storage of captured CO2 underground [5,6].Researchers exploring better applications of CCUS technology in the cement and con- [7,7,8].sulfoaluminate cement (CSA cement), as the third series of cement indeeloped in China, has become a highly promising low-carbon cement due to s of low calcination temperature, low consumption of limestone as raw easy wear resistance [9-12].In addition, CSA cement has high early impermeability and frost resistance and micro-expansion characteristics.n successfully applied in emergency repair and construction, marine conother projects [4,13,14].Ye'elimite (C4A3Š) and belite (C2S) are the main A cement: The former enables this type of cement to have quick hardening ly strength on account of its rapid hydration, and the latter provides later g to the C-S-H gel generated at the later age.Generally, the hydration of ccording to Equation (1) to generate monosulfate (C4AŠH12) and aluminum 3) gel.Under the circumstances of excessive water, C3AH6 may form acuation (2).Actually, during the manufacture of CSA cement, gypsum hydrite is used, and C4A3Š will react with calcium sulfate to generate ŠH32) and AH3 (Equation ( 3)).Moreover, the hydration of C2S tends to H and portlandite (CH) according to Equation (4).With the hydration of at the same time, C2S will react with AH3 to generate strȁtlingite (C2ASH8) .(1) e carbonation of CSA cement, most of the studies have focused on its meerty, such as compressive strength, expansion, etc. [15][16][17][18][19][20][21].For instance, ion, the mechanical property of CSA cement was improved as reported by , but it was also influenced by the water-to-cement ratio.Moreover, differn methods usually present various results, e.g., a carbonation chamber is or carbonation, and thus, the difference between the accelerated carbonavironmental carbonation can be investigated.Seo [20] studied CSA cement lemented with different amounts of MgO, and after hydration for 56 d, the carbonated for studying compressive strength; the result showed that the e of MgO was 10 wt.% for improvement of strength.By mixing with slag, l property of CSA cement can be promoted after being exposed to CO2 for ation [23].Regarding the microstructure during the carbonation of CSA s found that, after ettringite was entirely carbonated, the carbonation ly consisted of gypsum and calcium carbonate (in three polymorphs, i.e., ite and vaterite), which has been found with the XRD results reported by tlingite.

FT-IR Analysis
Figure 6 shows the FT-IR spectra of the carbonated samples at 10 s, 30 s, 1 min, 2 min, 5 min, 10 min, 15 min and 30 min.A signal O-H band positioned at 3436 cm −1 was visible in all of the samples, which represented the vibration frequencies characteristic of the gibbsite formed in the samples.With increasing carbonation time, the signal at 1410 cm −1 appeared more obvious, which was associated with C-O vibration in the calcite.In the samples carbonated for 10 s and 30 s, this signal was not observed in the spectra and further confirmed the XRD result that no calcite was generated at the earlier carbonation time.Meanwhile, the signals of C-O vibration at 875 cm −1 gradually sharpened with increasing carbonation time, which demonstrated the generation of calcite as well.Moreover, the C-O vibration located at various peaks represents the different morphologies of calcium carbonate, e.g., vibrations at 713 cm −1 and 745 cm −1 stand for the presence of aragonite and vaterite.Therefore, after being exposed to CO 2 , aragonite and vaterite were generated, owing to their characteristic peaks at the FT-IR spectra.In addition, Si-O vibration at 510 cm −1 was the characteristic peak of C 2 S, and its intensity began to weaken as the carbonation time prolonged, which further proved its carbonation as a result of calcium carbonate.S-O vibration positioned at 600 cm −1 , 615 cm −1 and 677 cm −1 was associated with anhydrite.Also, Al-O vibrations at 645 cm −1 and 690 cm −1 were the characteristic peaks of C 4 A 3 Š [40][41][42][43][44].

TGA Analysis
The TG-DTG curves of CSA cement at various carbonation times (30 s~30 min) are shown in Figure 7.The main mass loss in the curve between 300 °C and 800 °C was associated with the decomposition of all types of calcium carbonate [43,45,46].From the result of TG, the calcium carbonate in all of the carbonation samples mainly existed in crystalline morphology, and the amorphous form existed in small amounts, which was consistent with the XRD result.As for the small quantity of mass loss between 50 °C and 150 °C, it was considered the decomposition of gel water or crystal water.Obviously, with the increase in carbonation time, the content of calcium carbonate increased as well.The detailed mass loss between 300 °C and 800 °C is shown in Figure 8.The samples at the early stage of carbonation (30 s and 1 min) have relatively low mass loss, which illustrates that the carbonation degree was extremely low.The results can also be confirmed by the content of calcium carbonate and amorphous phase in the XRD results.It is obvious that the mass loss increased by 2.68% from 1 min to 2 min after carbonation and reached 4.49% at 2 min.The total amount of calcium carbonate reached

TGA Analysis
The TG-DTG curves of CSA cement at various carbonation times (30 s~30 min) are shown in Figure 7.The main mass loss in the curve between 300 • C and 800 • C was associated with the decomposition of all types of calcium carbonate [43,45,46].From the result of TG, the calcium carbonate in all of the carbonation samples mainly existed in crystalline morphology, and the amorphous form existed in small amounts, which was consistent with the XRD result.As for the small quantity of mass loss between 50 • C and 150 • C, it was considered the decomposition of gel water or crystal water.

TGA Analysis
The TG-DTG curves of CSA cement at various carbonation times (30 s~30 min) are shown in Figure 7.The main mass loss in the curve between 300 °C and 800 °C was associated with the decomposition of all types of calcium carbonate [43,45,46].From the result of TG, the calcium carbonate in all of the carbonation samples mainly existed in crystalline morphology, and the amorphous form existed in small amounts, which was consistent with the XRD result.As for the small quantity of mass loss between 50 °C and 150 °C, it was considered the decomposition of gel water or crystal water.Obviously, with the increase in carbonation time, the content of calcium carbonate increased as well.The detailed mass loss between 300 °C and 800 °C is shown in Figure 8.The samples at the early stage of carbonation (30 s and 1 min) have relatively low mass loss, which illustrates that the carbonation degree was extremely low.The results can also be confirmed by the content of calcium carbonate and amorphous phase in the XRD results.It is obvious that the mass loss increased by 2.68% from 1 min to 2 min after carbonation and reached 4.49% at 2 min.The total amount calcium carbonate reached Obviously, with the increase in carbonation time, the content of calcium carbonate increased as well.The detailed mass loss between 300 • C and 800 • C is shown in Figure 8.The samples at the early stage of carbonation (30 s and 1 min) have relatively low mass loss, which illustrates that the carbonation degree was extremely low.The results can also be confirmed by the content of calcium carbonate and amorphous phase in the XRD results.It is obvious that the mass loss increased by 2.68% from 1 min to 2 min after carbonation and reached 4.49% at 2 min.The total amount of calcium carbonate reached 6.55% at 30 min, which exactly indicated that the carbonation degree was improved as the carbonation time increased.
Buildings 2024, 14, x FOR PEER REVIEW 10 of 15 6.55% at 30 min, which exactly indicated that the carbonation degree was improved as the carbonation time increased.

SEM Analysis
Figure 9 shows the SEM images of the CSA samples at different carbonation times (5 min, 15 min, 30 min).From Figure 9(a-1), the square crystals along with a few needles were observed, which were related to the specific morphology of calcite and aragonite, respectively.Also, the hydration products covered the surface of the cement particles, and the carbonation products, including calcium carbonate crystals and some amorphous gels, were wrapped together (Figure 9(a-2)).When carbonated for 15 min, some agglomerated lamellas were visible, which was associated with the typical morphology of aluminum hydroxide (Figure 9(b-1)).In addition, the silica gel shape was found and formed a network, and the square calcite crystals could be observed with a larger particle size.The vaterite with a typically spherical morphology and the aragonite with the needle-like morphology were visible as well (Figure 9(b-2)).In the sample carbonated for 30 min, its surface was mostly covered by the square calcite crystals, bonding with some silica gel and aluminum hydroxide gel (Figure 9(c-1)).Different from the samples carbonated for 5 min and 15 min, the square calcite crystals were stacked and closed together when carbonated for 30 min, confirming the increasing amount of calcite obtained with the QXRD results (Figure 9(c-2)).

SEM Analysis
9 shows the SEM images of the CSA samples at different carbonation times (5 min, 15 min, 30 min).From Figure 9(a-1), the square crystals along with a few needles were observed, which were related to the specific morphology of calcite and aragonite, respectively.Also, the hydration products covered the surface of the cement particles, and the carbonation products, including calcium carbonate crystals and some amorphous gels, were wrapped together (Figure 9(a-2)).When carbonated for 15 min, some agglomerated lamellas were visible, which was associated with the typical morphology of aluminum hydroxide (Figure 9(b-1)).In addition, the silica gel shape was found and formed a network, and the square calcite crystals could be observed with a larger particle size.The vaterite with a typically spherical morphology and the aragonite with the needle-like morphology were visible as well (Figure 9(b-2)).In the sample carbonated for 30 min, its surface was mostly covered by the square calcite crystals, bonding with some silica gel and aluminum hydroxide gel (Figure 9(c-1)).Different from the samples carbonated for 5 min and 15 min, the square calcite crystals were stacked and closed together when carbonated for 30 min, confirming the increasing amount of calcite obtained with the QXRD results (Figure 9(c-2)).
Figure 10 shows the SEM images of the sample carbonated for 1 h and 2 h.The square calcite crystals and spherical vaterite crystals can be observed in Figure 10a, and they gathered on the surface of the unhydrated cement paste.Also, as observed in Figure 10b, a small pore was formed due to the hydration reaction, and the generated calcite crystals not only covered the surface of the unhydrated particles but also filled in the pores.This further revealed that the particles, which should have grown inside the pores, were carbonated directly inside the pore, and calcium carbonate was generated as a result.Furthermore, there were still unhydrated particles existing when carbonated for 1 h and 2 h, and this phenomenon was probably associated with C 4 A 3 Š in the cement.At the later age of wet carbonation, calcite was the predominant species with a clear contour and a better crystallization, and the morphology no longer changed with the increase in CO 2 .During the early stage, the particle size of calcium carbonate gradually enlarged and piled up; nevertheless, the morphology of the products no longer changed, owing to the abundant calcite generated later.later age of wet carbonation, calcite was the predominant species with a clear contour a a better crystallization, and the morphology no longer changed with the increase in C During the early stage, the particle size of calcium carbonate gradually enlarged a piled up; nevertheless, the morphology of the products no longer changed, owing to t abundant calcite generated later.

GEMS Analysis
The modeling method was conducted based on the hydration of CSA cement fi and then exposure to CO2.The thermodynamic modeling results are demonstrated Figure 11.It can be observed that, when exposed to CO2, the amounts of strȁtlingite a ettringite began to diminish, and carbon-ettringite was formed as one of the carbonati products of ettringite.As for the existence of strȁtlingite, it was considered that it w generated from the reaction of C2S and aluminum hydroxide, which was one of the h dration products of C4A3Š.With the increasing amount of CO2, C2S was gradually c bonated, and thus, it no longer reacted with aluminum hydroxide.It is worth noting th the thermodynamic modeling of CSA cement carbonation showed the occurrence mono-carbonate (C4AČH11), which was one of the carbonation products of monosulfa It can be attributed to the carbonation of a small amount of monosulfate generated fro the hydration products of C4A3Š and water.As is reported by Hargis, the carbonation monosulfate occurred according to Equations ( 6)-( 9), and when a small amount of C was added, monosulfate was carbonated according to Equation ( 6) to generate mon carbonate and ettringite.As an intermediate carbonation product of ettringite, c bon-ettringite only existed under the circumstance of CO2 ranging from 1 g to 9 g.W the content of ettringite diminished, gypsum, calcium carbonate and aluminum h droxide were generated as the ultimate carbonation products when CO2 was abunda [47].

GEMS Analysis
The modeling method was conducted based on the hydration of CSA cement first and then exposure to CO 2 .The thermodynamic modeling results are demonstrated in Figure 11.It can be observed that, when exposed to CO 2 , the amounts of str Carbon capture, utilization and storage (CCUS) technology has been proposed recently to prevent excessive carbon emissions, which includes three main processes: CO2 capture, utilization and storage.CO2 capture is the separation and collection of CO2 from factory emission sources; CO2 utilization refers to the use of captured CO2 for the manufacture of new products; CO2 storage is the storage of captured CO2 underground [5,6].Researchers are constantly exploring better applications of CCUS technology in the cement and concrete industry [7,7,8].Calcium sulfoaluminate cement (CSA cement), as the third series of cement independently developed in China, has become a highly promising low-carbon cement due to its advantages of low calcination temperature, low consumption of limestone as raw materials and easy wear resistance [9-12].In addition, CSA cement has high early strength, good impermeability and frost resistance and micro-expansion characteristics.It has also been successfully applied in emergency repair and construction, marine construction and other projects [4,13,14].Ye'elimite (C4A3Š) and belite (C2S) are the main minerals in CSA cement: The former enables this type of cement to have quick hardening speed and early strength on account of its rapid hydration, and the latter provides later strength owing to the C-S-H gel generated at the later age.Generally, the hydration of C4A3Š occurs according to Equation (1) to generate monosulfate (C4AŠH12) and aluminum hydroxide (AH3) gel.Under the circumstances of excessive water, C3AH6 may form according to Equation (2).Actually, during the manufacture of CSA cement, gypsum (CŠH2) or anhydrite is used, and C4A3Š will react with calcium sulfate to generate ettringite (C6AŠH32) and AH3 (Equation ( 3)).Moreover, the hydration of C2S tends to generate C-S-H and portlandite (CH) according to Equation ( 4).With the hydration of C4A3Š and C2S at the same time, C2S will react with AH3 to generate strȁtlingite (C2ASH8) (Equation ( 5)).(2) As for the carbonation of CSA cement, most of the studies have focused on its mechanical property, such as compressive strength, expansion, etc. [15][16][17][18][19][20][21].For instance, after carbonation, the mechanical property of CSA cement was improved as reported by Mechling [22], but it was also influenced by the water-to-cement ratio.Moreover, different carbonation methods usually present various results, e.g., a carbonation chamber is usually used for carbonation, and thus, the difference between the accelerated carbonation and the environmental carbonation can be investigated.Seo [20] studied CSA cement that was supplemented with different amounts of MgO, and after hydration for 56 d, the samples were carbonated for studying compressive strength; the result showed that the optimal dosage of MgO was 10 wt.% for improvement of strength.By mixing with slag, the mechanical property of CSA cement can be promoted after being exposed to CO2 for further carbonation [23].Regarding the microstructure during the carbonation of CSA cement, it was found that, after ettringite was entirely carbonated, the carbonation products mainly consisted of gypsum and calcium carbonate (in three polymorphs, i.e., calcite, aragonite and vaterite), which has been found with the XRD results reported by Daniela Gastaldia [19].Also, the carbonation of CSA cement supplemented with PC was tlingite and ettringite began to diminish, and carbon-ettringite was formed as one of the carbonation products of ettringite.As for the existence of str 024, 14, x FOR PEER REVIEW 2 of 15 Carbon capture, utilization and storage (CCUS) technology has been proposed recently to prevent excessive carbon emissions, which includes three main processes: CO2 capture, utilization and storage.CO2 capture is the separation and collection of CO2 from factory emission sources; CO2 utilization refers to the use of captured CO2 for the manufacture of new products; CO2 storage is the storage of captured CO2 underground [5,6].Researchers are constantly exploring better applications of CCUS technology in the cement and concrete industry [7,7,8].
Calcium sulfoaluminate cement (CSA cement), as the third series of cement independently developed in China, has become a highly promising low-carbon cement due to its advantages of low calcination temperature, low consumption of limestone as raw materials and easy wear resistance [9-12].In addition, CSA cement has high early strength, good impermeability and frost resistance and micro-expansion characteristics.It has also been successfully applied in emergency repair and construction, marine construction and other projects [4,13,14].Ye'elimite (C4A3Š) and belite (C2S) are the main minerals in CSA cement: The former enables this type of cement to have quick hardening speed and early strength on account of its rapid hydration, and the latter provides later strength owing to the C-S-H gel generated at the later age.Generally, the hydration of C4A3Š occurs according to Equation (1) to generate monosulfate (C4AŠH12) and aluminum hydroxide (AH3) gel.Under the circumstances of excessive water, C3AH6 may form according to Equation (2).Actually, during the manufacture of CSA cement, gypsum (CŠH2) or anhydrite is used, and C4A3Š will react with calcium sulfate to generate ettringite (C6AŠH32) and AH3 (Equation (3)).Moreover, the hydration of C2S tends to generate C-S-H and portlandite (CH) according to Equation (4).With the hydration of C4A3Š and C2S at the same time, C2S will react with AH3 to generate strȁtlingite (C2ASH8) (Equation ( 5)).
As for the carbonation of CSA cement, most of the studies have focused on its mechanical property, such as compressive strength, expansion, etc. [15][16][17][18][19][20][21].For instance, after carbonation, the mechanical property of CSA cement was improved as reported by Mechling [22], but it was also influenced by the water-to-cement ratio.Moreover, different carbonation methods usually present various results, e.g., a carbonation chamber is usually used for carbonation, and thus, the difference between the accelerated carbonation and the environmental carbonation can be investigated.Seo [20] studied CSA cement that was supplemented with different amounts of MgO, and after hydration for 56 d, the samples were carbonated for studying compressive strength; the result showed that the optimal dosage of MgO was 10 wt.% for improvement of strength.By mixing with slag, the mechanical property of CSA cement can be promoted after being exposed to CO2 for further carbonation [23].Regarding the microstructure during the carbonation of CSA cement, it was found that, after ettringite was entirely carbonated, the carbonation products mainly consisted of gypsum and calcium carbonate (in three polymorphs, i.e., calcite, aragonite and vaterite), which has been found with the XRD results reported by Daniela Gastaldia [19].Also, the carbonation of CSA cement supplemented with PC was tlingite, it was considered that it was generated from the reaction of C 2 S and aluminum hydroxide, which was one of the hydration products of C 4 A 3 Š.With the increasing amount of CO 2 , C 2 S was gradually carbonated, and thus, it no longer reacted with aluminum hydroxide.It is worth noting that the thermodynamic modeling of CSA cement carbonation showed the occurrence of mono-carbonate (C 4 A ČH 11 ), which was one of the carbonation products of monosulfate.It can be attributed to the carbonation of a small amount of monosulfate generated from the hydration products of C 4 A 3 Š and water.As is reported by Hargis, the carbonation of monosulfate occurred according to Equations ( 6)-(9), and when a small amount of CO 2 was added, monosulfate was carbonated according to Equation (6) to generate monocarbonate and ettringite.As an intermediate carbonation product of ettringite, carbon-ettringite only existed under the circumstance of CO 2 ranging from 1 g to 9 g.With the content of ettringite diminished, gypsum, calcium carbonate and aluminum hydroxide were generated as the ultimate carbonation products when CO 2 was abundant [47]

Figure 1 .
Figure 1.Particle size distribution of CSA cement.

Figure 1 .
Figure 1.Particle size distribution of CSA cement.

Figure 2 .
Figure 2. Schematic illustration of the wet-carbonation reaction device.

Figure 2 .
Figure 2. Schematic illustration of the wet-carbonation reaction device.

Figure 3 .
Figure 3. pH values of the solution at different carbonation times.

Figure 3 .
Figure 3. pH values of the solution at different carbonation times.

Figure 3 .
Figure 3. pH values of the solution at different carbonation times.

Figure 6 .
Figure 6.FT-IR curves of the CSA cement carbonation.

Figure 6 .
Figure 6.FT-IR curves of the CSA cement carbonation.

Figure 8 .
Figure 8. Mass loss between 300 °C and 800 °C of the carbonation samples.

Figure 8 .
Figure 8. Mass loss between 300 • C and 800 • C of the carbonation samples.

Figure 10 .
Figure 10.SEM images of the CSA cement carbonated for (a) 1 h and (b) 2 h.

Figure 10 .
Figure 10.SEM images of the CSA cement carbonated for (a) 1 h and (b) 2 h.

Table 1 .
Quantitative phase analysis results of CSA cement.

Figure 1 .
Particle size distribution of CSA cement.

Table 1 .
Quantitative phase analysis results of CSA cement.

Table 1 .
Quantitative phase analysis results of CSA cement.

Table 2 .
Quantitative phase analysis results for CSA cement at various carbonation times (wt.%).

Table 2 .
Quantitative phase analysis results for CSA cement at various carbonation times (wt.%).